data_njy1
_audit_creation_date              2016-10-28
_audit_creation_method
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_publ_contact_author_address      ?
_publ_contact_author_email        ?
_publ_contact_author_name         ''
_publ_contact_author_phone        ?
_publ_section_references
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2008). Acta Cryst. A64, 112-122.
;
_chemical_name_common             ?
_chemical_name_systematic         ?
_chemical_formula_moiety          '0.25(K24 Na16 O1488 Sm48 W348), 38(O)'
_chemical_formula_sum             'H172 K6 Na4 O410 Sm12 W87'
_chemical_formula_weight          24859.08
_chemical_absolute_configuration  ?
_chemical_melting_point           ?
loop_
  _atom_type_symbol
  _atom_type_description
  _atom_type_scat_dispersion_real
  _atom_type_scat_dispersion_imag
  _atom_type_scat_source
 'C' 'C' 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H' 'H' 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na' 'Na' 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O' 'O' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P' 'P' 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Nb' 'Nb' -2.0727 0.6215
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Sm' 'Sm' -0.1638 3.4418
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'W' 'W' -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K' 'K' 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system       'cubic'
_space_group_IT_number            220
_space_group_name_H-M_alt         'I -4 3 d'
_space_group_name_Hall            'I -4bd 2c 3'
loop_
  _space_group_symop_operation_xyz
 'x, y, z'
 '-x+1/2, -y, z+1/2'
 '-x, y+1/2, -z+1/2'
 'x+1/2, -y+1/2, -z'
 'z, x, y'
 'z+1/2, -x+1/2, -y'
 '-z+1/2, -x, y+1/2'
 '-z, x+1/2, -y+1/2'
 'y, z, x'
 '-y, z+1/2, -x+1/2'
 'y+1/2, -z+1/2, -x'
 '-y+1/2, -z, x+1/2'
 'y+1/4, x+1/4, z+1/4'
 '-y+1/4, -x+3/4, z+3/4'
 'y+3/4, -x+1/4, -z+3/4'
 '-y+3/4, x+3/4, -z+1/4'
 'x+1/4, z+1/4, y+1/4'
 '-x+3/4, z+3/4, -y+1/4'
 '-x+1/4, -z+3/4, y+3/4'
 'x+3/4, -z+1/4, -y+3/4'
 'z+1/4, y+1/4, x+1/4'
 'z+3/4, -y+1/4, -x+3/4'
 '-z+3/4, y+3/4, -x+1/4'
 '-z+1/4, -y+3/4, x+3/4'
 'x+1/2, y+1/2, z+1/2'
 '-x+1, -y+1/2, z+1'
 '-x+1/2, y+1, -z+1'
 'x+1, -y+1, -z+1/2'
 'z+1/2, x+1/2, y+1/2'
 'z+1, -x+1, -y+1/2'
 '-z+1, -x+1/2, y+1'
 '-z+1/2, x+1, -y+1'
 'y+1/2, z+1/2, x+1/2'
 '-y+1/2, z+1, -x+1'
 'y+1, -z+1, -x+1/2'
 '-y+1, -z+1/2, x+1'
 'y+3/4, x+3/4, z+3/4'
 '-y+3/4, -x+5/4, z+5/4'
 'y+5/4, -x+3/4, -z+5/4'
 '-y+5/4, x+5/4, -z+3/4'
 'x+3/4, z+3/4, y+3/4'
 '-x+5/4, z+5/4, -y+3/4'
 '-x+3/4, -z+5/4, y+5/4'
 'x+5/4, -z+3/4, -y+5/4'
 'z+3/4, y+3/4, x+3/4'
 'z+5/4, -y+3/4, -x+5/4'
 '-z+5/4, y+5/4, -x+3/4'
 '-z+3/4, -y+5/4, x+5/4'

_cell_length_a                    35.953(5)
_cell_length_b                    35.953(5)
_cell_length_c                    35.953(5)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      46475(19)
_cell_formula_units_Z             4
_cell_measurement_reflns_used     551
_cell_measurement_temperature     296(2)
_cell_measurement_theta_max       19.42
_cell_measurement_theta_min       2.53
_shelx_estimated_absorpt_T_max    0.065
_shelx_estimated_absorpt_T_min    0.038
_exptl_absorpt_coefficient_mu     23.076
_exptl_absorpt_correction_T_max   0.0654
_exptl_absorpt_correction_T_min   0.0380
_exptl_absorpt_correction_type    'Multi-scan'
_exptl_absorpt_process_details    SADABS
_exptl_absorpt_special_details    ?
_exptl_crystal_colour             colorless
_exptl_crystal_density_diffrn     3.553
_exptl_crystal_density_meas       .
_exptl_crystal_density_method     ?
_exptl_crystal_description        block
_exptl_crystal_F_000              43168
_exptl_crystal_size_max           0.41
_exptl_crystal_size_mid           0.32
_exptl_crystal_size_min           0.26
_exptl_transmission_factor_max    ?
_exptl_transmission_factor_min    ?
_diffrn_reflns_av_R_equivalents   0.1578
_diffrn_reflns_av_unetI/netI      0.0608
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max        30
_diffrn_reflns_limit_h_min        -42
_diffrn_reflns_limit_k_max        40
_diffrn_reflns_limit_k_min        -42
_diffrn_reflns_limit_l_max        42
_diffrn_reflns_limit_l_min        -42
_diffrn_reflns_number             114893
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full         25.086
_diffrn_reflns_theta_max          25.086
_diffrn_reflns_theta_min          1.602
_diffrn_ambient_temperature       296.15
_diffrn_detector_area_resol_mean  ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type   'CCD area detector'
_diffrn_measurement_method        'phi and omega scans'
_diffrn_radiation_monochromator   'graphite'
_diffrn_radiation_type            MoK\a
_diffrn_radiation_wavelength      0.71073
_diffrn_source                    ?
_reflns_Friedel_coverage          0.901
_reflns_Friedel_fraction_full     0.996
_reflns_Friedel_fraction_max      0.996
_reflns_number_gt                 5622
_reflns_number_total              6875
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression      'I > 2σ(I)'
_computing_cell_refinement        'SAINT v7.34A (Bruker, 200?)'
_computing_data_collection        ?
_computing_data_reduction         'SAINT v7.34A (Bruker, 200?)'
_computing_molecular_graphics     'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material   'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement   'ShelXL-2014/7 (Sheldrick, 2008)'
_computing_structure_solution     'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max          1.511
_refine_diff_density_min          -1.927
_refine_diff_density_rms          0.317
_refine_ls_abs_structure_details
;
 Flack x determined using 2373 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack    -0.003(11)
_refine_ls_extinction_coef        .
_refine_ls_extinction_method      none
_refine_ls_goodness_of_fit_ref    1.063
_refine_ls_hydrogen_treatment     undef
_refine_ls_matrix_type            full
_refine_ls_number_parameters      406
_refine_ls_number_reflns          6875
_refine_ls_number_restraints      156
_refine_ls_R_factor_all           0.0643
_refine_ls_R_factor_gt            0.0398
_refine_ls_restrained_S_all       1.059
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0484P)²+995.6187P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme       calc
_refine_ls_wR_factor_gt           0.0882
_refine_ls_wR_factor_ref          0.1003
_refine_special_details           ?
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O2W) \\sim Ueq, Uanis(O3W) \\sim Ueq, Uanis(O4) \\sim Ueq, Uanis(O5)
\\sim Ueq, Uanis(O6) \\sim Ueq, Uanis(O8) \\sim Ueq, Uanis(O14) \\sim Ueq,
Uanis(O22) \\sim Ueq, Uanis(O24) \\sim Ueq, Uanis(O11) \\sim Ueq, Uanis(O23)
\\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O3) \\sim Ueq, Uanis(O12) \\sim Ueq, Uanis(O21) \\sim Ueq, Uanis(O9)
\\sim Ueq, Uanis(O10) \\sim Ueq, Uanis(O19) \\sim Ueq, Uanis(O8W) \\sim Ueq,
Uanis(O9W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O1) \\sim Ueq, Uanis(O9) \\sim Ueq, Uanis(O15) \\sim Ueq, Uanis(O20)
\\sim Ueq, Uanis(O4W) \\sim Ueq, Uanis(O5W) \\sim Ueq, Uanis(O7W) \\sim Ueq,
Uanis(O10W) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
2. Others
 Fixed Sof: O7W(0.5) O8W(0.5) O9W(0.16667) O10W(0.5)
;
_atom_sites_solution_hydrogens    .
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    ?
loop_
  _atom_site_label
  _atom_site_type_symbol
  _atom_site_fract_x
  _atom_site_fract_y
  _atom_site_fract_z
  _atom_site_U_iso_or_equiv
  _atom_site_adp_type
  _atom_site_occupancy
  _atom_site_site_symmetry_order
  _atom_site_calc_flag
  _atom_site_refinement_flags_posn
  _atom_site_refinement_flags_adp
  _atom_site_refinement_flags_occupancy
  _atom_site_disorder_assembly
  _atom_site_disorder_group
 W1 W 0.5000 0.2500 0.1250 0.0085(5) Uani 1 4 d S T P . .
 W2 W 0.54597(3) 0.15162(3) 0.06750(3) 0.0134(3) Uani 1 1 d . . . . .
 W3 W 0.60189(3) 0.22258(3) 0.06540(3) 0.0133(3) Uani 1 1 d . . . . .
 W4 W 0.61260(3) 0.15417(4) 0.00005(4) 0.0218(3) Uani 1 1 d . . . . .
 W5 W 0.54907(4) 0.08772(4) 0.00440(4) 0.0273(3) Uani 1 1 d . . . . .
 W6 W 0.53188(4) 0.15711(4) -0.05076(4) 0.0301(4) Uani 1 1 d . . . . .
 W7 W 0.58763(5) 0.22892(4) -0.05407(4) 0.0344(4) Uani 1 1 d . . . . .
 W8 W 0.66058(4) 0.23283(4) -0.00114(4) 0.0330(4) Uani 1 1 d . . . . .
 Sm1 Sm 0.58123(4) 0.18376(4) 0.16909(4) 0.0136(3) Uani 1 1 d . . . . .
 K1 K 0.5000 0.2500 0.0201(3) 0.033(3) Uani 1 2 d S T P . .
 Na1 Na 0.5088(6) -0.0088(6) 0.0088(6) 0.063(10) Uani 1 3 d S T P . .
 O1 O 0.5321(5) 0.2247(5) 0.1532(5) 0.011(4) Uani 1 1 d . U . . .
 O2 O 0.5574(6) 0.1512(5) 0.1152(5) 0.019(5) Uani 1 1 d . . . . .
 O3 O 0.4976(5) 0.1505(5) 0.0648(5) 0.013(4) Uani 1 1 d . U . . .
 O4 O 0.5513(5) 0.2052(5) 0.0590(5) 0.018(5) Uani 1 1 d . U . . .
 O5 O 0.6054(5) 0.1625(5) 0.0513(5) 0.014(4) Uani 1 1 d . U . . .
 O6 O 0.5575(6) 0.1014(6) 0.0571(6) 0.025(5) Uani 1 1 d . U . . .
 O7 O 0.5505(6) 0.1455(6) 0.0069(6) 0.024(5) Uani 1 1 d . . . . .
 O8 O 0.6070(5) 0.2133(5) 0.1124(5) 0.018(4) Uani 1 1 d . U . . .
 O9 O 0.5926(5) 0.2704(5) 0.0622(5) 0.011(4) Uani 1 1 d . U . . .
 O10 O 0.6535(5) 0.2215(6) 0.0527(6) 0.025(5) Uani 1 1 d . U . . .
 O11 O 0.6052(6) 0.2168(6) 0.0055(5) 0.021(5) Uani 1 1 d . U . . .
 O12 O 0.6105(6) 0.1044(6) -0.0027(6) 0.027(5) Uani 1 1 d . U . . .
 O13 O 0.6597(5) 0.1660(6) -0.0042(6) 0.032(6) Uani 1 1 d . . . . .
 O14 O 0.5940(6) 0.1666(6) -0.0472(6) 0.030(5) Uani 1 1 d . U . . .
 O15 O 0.5021(5) 0.0797(6) 0.0103(6) 0.025(5) Uani 1 1 d . U . . .
 O16 O 0.5464(7) 0.1043(7) -0.0473(6) 0.040(6) Uani 1 1 d . . . . .
 O17 O 0.5705(7) 0.0405(7) 0.0211(8) 0.050(7) Uani 1 1 d . . . . .
 O18 O 0.5649(8) 0.0423(8) -0.0182(9) 0.061(8) Uani 1 1 d . . . . .
 O19 O 0.4854(6) 0.1518(7) -0.0387(6) 0.041(6) Uani 1 1 d . U . . .
 O20 O 0.5319(6) 0.1585(7) -0.0996(6) 0.039(6) Uani 1 1 d . U . . .
 O21 O 0.5394(6) 0.2088(7) -0.0395(6) 0.036(6) Uani 1 1 d . U . . .
 O22 O 0.5841(7) 0.2277(7) -0.1018(6) 0.047(7) Uani 1 1 d . U . . .
 O23 O 0.5767(8) 0.2754(7) -0.0428(7) 0.050(7) Uani 1 1 d . U . . .
 O24 O 0.6416(6) 0.2282(6) -0.0526(6) 0.034(6) Uani 1 1 d . U . . .
 O25 O 0.6563(8) 0.2813(6) 0.0023(8) 0.050(7) Uani 1 1 d . . . . .
 O26 O 0.7065(7) 0.2293(9) -0.0285(9) 0.057(8) Uani 1 1 d . . . . .
 O27 O 0.7125(7) 0.2250(8) 0.0127(10) 0.064(9) Uani 1 1 d . . . . .
 O1W O 0.6352(9) 0.1417(8) 0.1400(9) 0.069(9) Uani 1 1 d . . . . .
 O2W O 0.5857(7) 0.1218(7) 0.1997(7) 0.046(7) Uani 1 1 d . U . . .
 O3W O 0.5627(7) 0.1988(7) 0.2328(6) 0.039(6) Uani 1 1 d . U . . .
 O4W O 0.6426(7) 0.1887(7) 0.2026(8) 0.052(7) Uani 1 1 d . U . . .
 O5W O 0.6905(6) 0.2022(7) 0.1199(7) 0.042(6) Uani 1 1 d . U . . .
 O6W O 0.7500 0.2929(11) 0.0000 0.089(18) Uani 1 2 d S T P . .
 O7W O 0.4332(13) 0.1663(13) -0.0951(12) 0.038(12) Uani 0.5 1 d . U . . .
 O8W O 0.5860(15) 0.0697(13) 0.1266(13) 0.046(13) Uani 0.5 1 d . U . . .
 O9W O 0.450(2) 0.050(2) -0.050(2) 0.10(2) Uani 0.5 3 d S TU P . .
 O10W O 0.697(2) 0.160(2) 0.070(2) 0.10(3) Uani 0.5 1 d . U . . .


_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
  _geom_bond_atom_site_label_1
  _geom_bond_atom_site_label_2
  _geom_bond_distance
  _geom_bond_site_symmetry_2
  _geom_bond_publ_flag
 W1 K1 3.771(11) . ?
 W1 K1 3.771(11) 39_454 ?
 W1 O1 1.785(17) 39_454 ?
 W1 O1 1.785(17) 16_545 ?
 W1 O1 1.785(17) 26_554 ?
 W1 O1 1.785(17) . ?
 W2 W5 3.2309(17) . ?
 W2 O2 1.762(18) . ?
 W2 O3 1.744(17) . ?
 W2 O4 1.959(19) . ?
 W2 O5 2.250(18) . ?
 W2 O6 1.89(2) . ?
 W2 O7 2.19(2) . ?
 W3 W8 3.2112(18) . ?
 W3 K1 4.128(4) . ?
 W3 O4 1.938(19) . ?
 W3 O5 2.222(18) . ?
 W3 O8 1.733(18) . ?
 W3 O9 1.754(17) . ?
 W3 O10 1.911(19) . ?
 W3 O11 2.168(19) . ?
 W4 O5 1.885(19) . ?
 W4 O7 2.27(2) . ?
 W4 O11 2.28(2) . ?
 W4 O12 1.79(2) . ?
 W4 O13 1.75(2) . ?
 W4 O14 1.88(2) . ?
 W5 O6 1.98(2) . ?
 W5 O7 2.08(2) . ?
 W5 O12 2.30(2) . ?
 W5 O15 1.72(2) . ?
 W5 O16 1.96(2) . ?
 W5 O17 1.96(3) . ?
 W5 O18 1.91(3) . ?
 W6 O7 2.22(2) . ?
 W6 O14 2.26(2) . ?
 W6 O16 1.97(2) . ?
 W6 O19 1.74(2) . ?
 W6 O20 1.76(2) . ?
 W6 O21 1.92(2) . ?
 W7 O11 2.27(2) . ?
 W7 O14 2.27(2) . ?
 W7 O21 1.95(2) . ?
 W7 O22 1.72(2) . ?
 W7 O23 1.76(2) . ?
 W7 O24 1.94(2) . ?
 W8 O10 1.99(2) . ?
 W8 O11 2.09(2) . ?
 W8 O13 2.40(2) . ?
 W8 O24 1.98(2) . ?
 W8 O25 1.75(2) . ?
 W8 O26 1.93(2) . ?
 W8 O27 1.95(3) . ?
 Sm1 K1 4.356(6) 39_454 ?
 Sm1 O1 2.369(17) . ?
 Sm1 O2 2.422(18) . ?
 Sm1 O3 2.455(17) 16_545 ?
 Sm1 O8 2.477(19) . ?
 Sm1 O9 2.478(17) 39_454 ?
 Sm1 O1W 2.67(3) . ?
 Sm1 O2W 2.49(2) . ?
 Sm1 O3W 2.45(2) . ?
 Sm1 O4W 2.52(2) . ?
 K1 W3 4.128(4) 26_554 ?
 K1 Sm1 4.356(6) 16_545 ?
 K1 O1 3.13(2) 39_454 ?
 K1 O1 3.13(2) 16_545 ?
 K1 O4 2.819(19) 26_554 ?
 K1 O4 2.819(19) . ?
 K1 O21 2.97(2) 26_554 ?
 K1 O21 2.97(2) . ?
 K1 O3W 2.91(3) 16_545 ?
 K1 O3W 2.91(3) 39_454 ?
 Na1 O17 2.87(3) 6 ?
 Na1 O17 2.87(3) . ?
 Na1 O17 2.87(3) 12_554 ?
 Na1 O18 2.90(3) 6 ?
 Na1 O18 2.90(3) . ?
 Na1 O18 2.90(3) 12_554 ?
 O1 K1 3.13(2) 39_454 ?
 O3 Sm1 2.455(17) 39_454 ?
 O9 Sm1 2.478(17) 16_545 ?
 O17 O18 1.43(4) . ?
 O26 O27 1.50(4) . ?
 O3W K1 2.91(3) 39_454 ?

loop_
  _geom_angle_atom_site_label_1
  _geom_angle_atom_site_label_2
  _geom_angle_atom_site_label_3
  _geom_angle
  _geom_angle_site_symmetry_1
  _geom_angle_site_symmetry_3
  _geom_angle_publ_flag
 K1 W1 K1 180.0 39_454 . ?
 O1 W1 K1 55.4(6) 16_545 . ?
 O1 W1 K1 55.4(6) . 39_454 ?
 O1 W1 K1 55.4(6) 39_454 . ?
 O1 W1 K1 124.6(6) 26_554 . ?
 O1 W1 K1 124.6(6) 39_454 39_454 ?
 O1 W1 K1 124.6(6) . . ?
 O1 W1 K1 124.6(6) 16_545 39_454 ?
 O1 W1 K1 55.4(6) 26_554 39_454 ?
 O1 W1 O1 108.8(6) 16_545 26_554 ?
 O1 W1 O1 108.8(6) 39_454 26_554 ?
 O1 W1 O1 110.9(11) 26_554 . ?
 O1 W1 O1 110.9(11) 39_454 16_545 ?
 O1 W1 O1 108.8(6) 16_545 . ?
 O1 W1 O1 108.8(6) 39_454 . ?
 O2 W2 W5 131.9(6) . . ?
 O2 W2 O4 97.9(8) . . ?
 O2 W2 O5 91.8(8) . . ?
 O2 W2 O6 97.6(9) . . ?
 O2 W2 O7 161.2(8) . . ?
 O3 W2 W5 88.8(6) . . ?
 O3 W2 O2 106.6(9) . . ?
 O3 W2 O4 96.4(8) . . ?
 O3 W2 O5 159.8(7) . . ?
 O3 W2 O6 100.6(9) . . ?
 O3 W2 O7 91.0(8) . . ?
 O4 W2 W5 125.9(6) . . ?
 O4 W2 O5 72.3(7) . . ?
 O4 W2 O7 86.4(8) . . ?
 O5 W2 W5 84.8(5) . . ?
 O6 W2 W5 34.3(6) . . ?
 O6 W2 O4 152.5(8) . . ?
 O6 W2 O5 84.7(8) . . ?
 O6 W2 O7 72.0(8) . . ?
 O7 W2 W5 39.6(5) . . ?
 O7 W2 O5 71.9(7) . . ?
 W8 W3 K1 105.18(14) . . ?
 O4 W3 W8 124.5(6) . . ?
 O4 W3 K1 36.6(6) . . ?
 O4 W3 O5 73.3(7) . . ?
 O4 W3 O11 84.4(8) . . ?
 O5 W3 W8 84.5(5) . . ?
 O5 W3 K1 101.1(5) . . ?
 O8 W3 W8 132.8(6) . . ?
 O8 W3 K1 121.7(7) . . ?
 O8 W3 O4 98.8(8) . . ?
 O8 W3 O5 91.7(8) . . ?
 O8 W3 O9 105.8(9) . . ?
 O8 W3 O10 97.3(9) . . ?
 O8 W3 O11 161.0(8) . . ?
 O9 W3 W8 87.9(6) . . ?
 O9 W3 K1 64.7(6) . . ?
 O9 W3 O4 97.5(8) . . ?
 O9 W3 O5 161.5(7) . . ?
 O9 W3 O10 100.9(8) . . ?
 O9 W3 O11 92.2(8) . . ?
 O10 W3 W8 35.5(7) . . ?
 O10 W3 K1 140.5(7) . . ?
 O10 W3 O4 151.2(8) . . ?
 O10 W3 O5 82.5(8) . . ?
 O10 W3 O11 73.0(8) . . ?
 O11 W3 W8 40.0(5) . . ?
 O11 W3 K1 71.3(5) . . ?
 O11 W3 O5 71.2(7) . . ?
 O5 W4 O7 77.3(7) . . ?
 O5 W4 O11 75.1(7) . . ?
 O7 W4 O11 90.7(7) . . ?
 O12 W4 O5 102.0(9) . . ?
 O12 W4 O7 80.1(8) . . ?
 O12 W4 O11 170.7(8) . . ?
 O12 W4 O14 99.9(10) . . ?
 O13 W4 O5 100.3(9) . . ?
 O13 W4 O7 173.7(9) . . ?
 O13 W4 O11 83.1(9) . . ?
 O13 W4 O12 106.2(10) . . ?
 O13 W4 O14 101.9(10) . . ?
 O14 W4 O5 142.9(8) . . ?
 O14 W4 O7 77.4(9) . . ?
 O14 W4 O11 78.5(8) . . ?
 O6 W5 W2 32.5(6) . . ?
 O6 W5 O7 72.9(8) . . ?
 O6 W5 O12 84.0(8) . . ?
 O7 W5 W2 42.3(6) . . ?
 O7 W5 O12 73.8(7) . . ?
 O12 W5 W2 85.7(5) . . ?
 O15 W5 W2 89.9(6) . . ?
 O15 W5 O6 94.2(9) . . ?
 O15 W5 O7 100.7(9) . . ?
 O15 W5 O12 174.4(8) . . ?
 O15 W5 O16 96.9(10) . . ?
 O15 W5 O17 101.7(11) . . ?
 O15 W5 O18 101.7(11) . . ?
 O16 W5 W2 116.7(7) . . ?
 O16 W5 O6 147.3(9) . . ?
 O16 W5 O7 74.9(9) . . ?
 O16 W5 O12 82.1(10) . . ?
 O16 W5 O17 125.1(11) . . ?
 O17 W5 W2 114.5(8) . . ?
 O17 W5 O6 82.1(10) . . ?
 O17 W5 O7 147.4(9) . . ?
 O17 W5 O12 83.3(9) . . ?
 O18 W5 W2 156.4(10) . . ?
 O18 W5 O6 125.0(12) . . ?
 O18 W5 O7 149.8(11) . . ?
 O18 W5 O12 83.6(10) . . ?
 O18 W5 O16 82.6(12) . . ?
 O18 W5 O17 43.3(12) . . ?
 O7 W6 O14 71.2(7) . . ?
 O16 W6 O7 71.4(8) . . ?
 O16 W6 O14 83.1(10) . . ?
 O19 W6 O7 92.1(10) . . ?
 O19 W6 O14 162.2(9) . . ?
 O19 W6 O16 97.6(12) . . ?
 O19 W6 O20 104.6(11) . . ?
 O19 W6 O21 101.0(11) . . ?
 O20 W6 O7 160.0(9) . . ?
 O20 W6 O14 93.0(9) . . ?
 O20 W6 O16 95.2(10) . . ?
 O20 W6 O21 100.5(11) . . ?
 O21 W6 O7 86.8(9) . . ?
 O21 W6 O14 72.7(9) . . ?
 O21 W6 O16 151.7(10) . . ?
 O14 W7 O11 71.4(7) . . ?
 O21 W7 O11 85.6(9) . . ?
 O21 W7 O14 72.2(9) . . ?
 O22 W7 O11 162.6(10) . . ?
 O22 W7 O14 95.2(10) . . ?
 O22 W7 O21 101.0(11) . . ?
 O22 W7 O23 103.7(12) . . ?
 O22 W7 O24 95.8(11) . . ?
 O23 W7 O11 91.6(10) . . ?
 O23 W7 O14 159.1(10) . . ?
 O23 W7 O21 95.2(11) . . ?
 O23 W7 O24 103.3(12) . . ?
 O24 W7 O11 72.2(8) . . ?
 O24 W7 O14 83.2(9) . . ?
 O24 W7 O21 151.2(10) . . ?
 O10 W8 W3 33.8(6) . . ?
 O10 W8 O11 73.2(8) . . ?
 O10 W8 O13 80.7(8) . . ?
 O11 W8 W3 42.0(5) . . ?
 O11 W8 O13 73.5(7) . . ?
 O13 W8 W3 84.9(5) . . ?
 O24 W8 W3 117.4(6) . . ?
 O24 W8 O10 147.7(9) . . ?
 O24 W8 O11 75.7(8) . . ?
 O24 W8 O13 82.4(9) . . ?
 O25 W8 W3 90.3(8) . . ?
 O25 W8 O10 97.1(11) . . ?
 O25 W8 O11 100.5(11) . . ?
 O25 W8 O13 174.0(10) . . ?
 O25 W8 O24 96.8(12) . . ?
 O25 W8 O26 100.2(12) . . ?
 O25 W8 O27 102.1(13) . . ?
 O26 W8 W3 159.4(9) . . ?
 O26 W8 O10 126.3(11) . . ?
 O26 W8 O11 149.1(11) . . ?
 O26 W8 O13 85.5(10) . . ?
 O26 W8 O24 79.2(11) . . ?
 O26 W8 O27 45.6(12) . . ?
 O27 W8 W3 115.0(10) . . ?
 O27 W8 O10 81.2(11) . . ?
 O27 W8 O11 147.6(11) . . ?
 O27 W8 O13 83.2(10) . . ?
 O27 W8 O24 123.8(11) . . ?
 O1 Sm1 K1 44.1(4) . 39_454 ?
 O1 Sm1 O2 81.0(6) . . ?
 O1 Sm1 O3 71.1(6) . 16_545 ?
 O1 Sm1 O8 79.2(6) . . ?
 O1 Sm1 O9 69.2(6) . 39_454 ?
 O1 Sm1 O1W 143.0(8) . . ?
 O1 Sm1 O2W 135.3(7) . . ?
 O1 Sm1 O3W 83.5(7) . . ?
 O1 Sm1 O4W 136.4(7) . . ?
 O2 Sm1 K1 115.4(5) . 39_454 ?
 O2 Sm1 O3 137.3(6) . 16_545 ?
 O2 Sm1 O8 71.4(6) . . ?
 O2 Sm1 O9 73.7(6) . 39_454 ?
 O2 Sm1 O1W 70.8(8) . . ?
 O2 Sm1 O2W 86.8(8) . . ?
 O2 Sm1 O3W 139.5(7) . . ?
 O2 Sm1 O4W 136.6(8) . . ?
 O3 Sm1 K1 63.3(4) 16_545 39_454 ?
 O3 Sm1 O8 72.1(6) 16_545 . ?
 O3 Sm1 O9 122.1(6) 16_545 39_454 ?
 O3 Sm1 O1W 115.2(9) 16_545 . ?
 O3 Sm1 O2W 135.6(8) 16_545 . ?
 O3 Sm1 O4W 65.6(7) 16_545 . ?
 O8 Sm1 K1 115.4(5) . 39_454 ?
 O8 Sm1 O9 135.8(6) . 39_454 ?
 O8 Sm1 O1W 69.5(9) . . ?
 O8 Sm1 O2W 136.3(8) . . ?
 O8 Sm1 O4W 92.0(8) . . ?
 O9 Sm1 K1 58.8(4) 39_454 39_454 ?
 O9 Sm1 O1W 122.1(8) 39_454 . ?
 O9 Sm1 O2W 66.1(7) 39_454 . ?
 O9 Sm1 O4W 132.1(8) 39_454 . ?
 O1W Sm1 K1 172.8(6) . 39_454 ?
 O2W Sm1 K1 108.1(6) . 39_454 ?
 O2W Sm1 O1W 67.7(9) . . ?
 O2W Sm1 O4W 78.2(8) . . ?
 O3W Sm1 K1 39.4(6) . 39_454 ?
 O3W Sm1 O3 69.3(7) . 16_545 ?
 O3W Sm1 O8 141.0(7) . . ?
 O3W Sm1 O9 65.8(7) . 39_454 ?
 O3W Sm1 O1W 133.5(9) . . ?
 O3W Sm1 O2W 78.5(9) . . ?
 O3W Sm1 O4W 77.0(9) . . ?
 O4W Sm1 K1 108.0(7) . 39_454 ?
 O4W Sm1 O1W 65.8(9) . . ?
 W1 K1 W3 66.77(14) . . ?
 W1 K1 W3 66.77(14) . 26_554 ?
 W1 K1 Sm1 59.89(12) . 16_545 ?
 W3 K1 W3 133.5(3) . 26_554 ?
 W3 K1 Sm1 97.30(15) 26_554 16_545 ?
 W3 K1 Sm1 58.47(8) . 16_545 ?
 O1 K1 W1 28.1(3) 39_454 . ?
 O1 K1 W1 28.1(3) 16_545 . ?
 O1 K1 W3 58.8(3) 39_454 26_554 ?
 O1 K1 W3 79.7(4) 39_454 . ?
 O1 K1 W3 79.7(4) 16_545 26_554 ?
 O1 K1 W3 58.8(3) 16_545 . ?
 O1 K1 Sm1 87.9(4) 39_454 16_545 ?
 O1 K1 Sm1 31.8(3) 16_545 16_545 ?
 O1 K1 O1 56.1(6) 16_545 39_454 ?
 O4 K1 W1 60.3(4) 26_554 . ?
 O4 K1 W1 60.3(4) . . ?
 O4 K1 W3 121.4(5) . 26_554 ?
 O4 K1 W3 24.2(4) 26_554 26_554 ?
 O4 K1 W3 24.2(4) . . ?
 O4 K1 W3 121.4(5) 26_554 . ?
 O4 K1 Sm1 77.1(4) . 16_545 ?
 O4 K1 Sm1 74.1(4) 26_554 16_545 ?
 O4 K1 O1 65.4(5) 26_554 39_454 ?
 O4 K1 O1 62.7(5) 26_554 16_545 ?
 O4 K1 O1 62.7(5) . 39_454 ?
 O4 K1 O1 65.4(5) . 16_545 ?
 O4 K1 O4 120.5(9) 26_554 . ?
 O4 K1 O21 76.2(6) 26_554 26_554 ?
 O4 K1 O21 163.0(7) 26_554 . ?
 O4 K1 O21 76.2(6) . . ?
 O4 K1 O21 163.0(7) . 26_554 ?
 O4 K1 O3W 92.7(6) . 16_545 ?
 O4 K1 O3W 92.7(6) 26_554 39_454 ?
 O4 K1 O3W 89.4(6) . 39_454 ?
 O4 K1 O3W 89.4(6) 26_554 16_545 ?
 O21 K1 W1 136.3(5) 26_554 . ?
 O21 K1 W1 136.3(5) . . ?
 O21 K1 W3 75.1(5) 26_554 26_554 ?
 O21 K1 W3 145.9(5) . 26_554 ?
 O21 K1 W3 75.1(5) . . ?
 O21 K1 W3 145.9(5) 26_554 . ?
 O21 K1 Sm1 106.8(5) 26_554 16_545 ?
 O21 K1 Sm1 115.9(5) . 16_545 ?
 O21 K1 O1 126.3(6) 26_554 16_545 ?
 O21 K1 O1 133.1(6) . 16_545 ?
 O21 K1 O1 126.3(6) . 39_454 ?
 O21 K1 O1 133.1(6) 26_554 39_454 ?
 O21 K1 O21 87.4(9) 26_554 . ?
 O3W K1 W1 92.1(5) 16_545 . ?
 O3W K1 W1 92.1(5) 39_454 . ?
 O3W K1 W3 68.8(5) 16_545 . ?
 O3W K1 W3 68.8(5) 39_454 26_554 ?
 O3W K1 W3 113.0(5) 39_454 . ?
 O3W K1 W3 113.0(5) 16_545 26_554 ?
 O3W K1 Sm1 152.0(6) 39_454 16_545 ?
 O3W K1 Sm1 32.2(4) 16_545 16_545 ?
 O3W K1 O1 64.0(6) 16_545 16_545 ?
 O3W K1 O1 120.1(6) 16_545 39_454 ?
 O3W K1 O1 120.1(6) 39_454 16_545 ?
 O3W K1 O1 64.0(6) 39_454 39_454 ?
 O3W K1 O21 83.6(7) 16_545 26_554 ?
 O3W K1 O21 83.6(7) 39_454 . ?
 O3W K1 O21 93.3(7) 16_545 . ?
 O3W K1 O21 93.3(7) 39_454 26_554 ?
 O3W K1 O3W 175.8(10) 39_454 16_545 ?
 O17 Na1 O17 116.9(5) 6 . ?
 O17 Na1 O17 116.9(5) 6 12_554 ?
 O17 Na1 O17 116.9(5) 12_554 . ?
 O17 Na1 O18 100.1(7) 6 . ?
 O17 Na1 O18 141.8(7) 12_554 . ?
 O17 Na1 O18 141.8(7) . 6 ?
 O17 Na1 O18 28.6(8) 12_554 12_554 ?
 O17 Na1 O18 28.6(8) . . ?
 O17 Na1 O18 100.1(7) 12_554 6 ?
 O17 Na1 O18 28.6(8) 6 6 ?
 O17 Na1 O18 100.1(7) . 12_554 ?
 O17 Na1 O18 141.8(7) 6 12_554 ?
 O18 Na1 O18 117.6(5) 6 . ?
 O18 Na1 O18 117.6(5) 12_554 . ?
 O18 Na1 O18 117.6(5) 6 12_554 ?
 W1 O1 Sm1 159.4(10) . . ?
 W1 O1 K1 96.5(7) . 39_454 ?
 Sm1 O1 K1 104.1(6) . 39_454 ?
 W2 O2 Sm1 148.9(10) . . ?
 W2 O3 Sm1 156.0(10) . 39_454 ?
 W2 O4 K1 125.1(8) . . ?
 W3 O4 W2 113.0(9) . . ?
 W3 O4 K1 119.2(8) . . ?
 W3 O5 W2 93.2(7) . . ?
 W4 O5 W2 110.8(9) . . ?
 W4 O5 W3 112.7(8) . . ?
 W2 O6 W5 113.1(11) . . ?
 W2 O7 W4 99.7(8) . . ?
 W2 O7 W6 152.4(10) . . ?
 W5 O7 W2 98.2(9) . . ?
 W5 O7 W4 99.1(8) . . ?
 W5 O7 W6 98.0(8) . . ?
 W6 O7 W4 99.8(8) . . ?
 W3 O8 Sm1 147.7(10) . . ?
 W3 O9 Sm1 156.9(9) . 16_545 ?
 W3 O10 W8 110.6(10) . . ?
 W3 O11 W4 100.7(8) . . ?
 W3 O11 W7 154.4(10) . . ?
 W7 O11 W4 98.1(7) . . ?
 W8 O11 W3 98.0(8) . . ?
 W8 O11 W4 98.7(8) . . ?
 W8 O11 W7 96.0(8) . . ?
 W4 O12 W5 107.1(9) . . ?
 W4 O13 W8 104.6(10) . . ?
 W4 O14 W6 111.5(10) . . ?
 W4 O14 W7 111.6(11) . . ?
 W6 O14 W7 92.5(8) . . ?
 W5 O16 W6 111.4(11) . . ?
 W5 O17 Na1 100.6(12) . . ?
 O18 O17 W5 66.6(17) . . ?
 O18 O17 Na1 76.6(16) . . ?
 W5 O18 Na1 101.0(11) . . ?
 O17 O18 W5 70.1(15) . . ?
 O17 O18 Na1 74.8(17) . . ?
 W6 O21 W7 115.3(11) . . ?
 W6 O21 K1 124.6(10) . . ?
 W7 O21 K1 115.7(10) . . ?
 W7 O24 W8 111.6(9) . . ?
 O27 O26 W8 68.1(14) . . ?
 O26 O27 W8 66.3(16) . . ?
 Sm1 O3W K1 108.4(9) . 39_454 ?

_shelx_SHELXL_version_number      '2014/7'
_olex2_submission_special_instructions 'No special instructions were received'

